### Annihilation of Edge Dislocations in SmA Liquid Crystals

M. Ambroˇziˇc1,2_{, S.Kralj}2,3_{, T.J. Sluckin}4_{, S.ˇ}_{Zumer}5,3_{, and D. Svenˇsek}5

1_{Engineering Ceramics Department,}*Joˇzef Stefan Institute,*

*Jamova 39, 1000 Ljubljana, Slovenia*

2_{Laboratory of Physics of Complex Systems,}*Faculty of Education,*

*University of Maribor,*

*Koroˇska 160, 2000 Maribor, Slovenia*

3_{Condensed Matter Physics Department,}*Joˇzef Stefan Institute,*

*Jamova 39, 1000 Ljubljana, Slovenia*

4_{School of Mathematics,}*University of Southampton,*

*Southampton SO17 1BJ, United Kingdom*

5_{Department of Physics,}*Faculty of Mathematics and Physics,*

*University of Ljubljana, Jadranska 19,*

*1000 Ljubljana, Slovenia*

### Abstract

This paper presents a theoretical study of the annihilation of edge dislocations in the same smectic
plane in a bulk smectic A phase. We use a time-dependent Landau-Ginzburg approach where
the smectic ordering is described by the complex order parameter *ψ(−→r , t) =ηeiφ*_{. This quantity}

allows both the degree of layering and the position of the layers to be monitored. We are able
to follow both pre-collision and post-collision regimes, and distinguish different early and late
behaviors within these regimes. The early pre-collision regime is driven by changes in the *φ(−→r*)
configuration. The relative velocity of the defects is approximately inversely proportional to the
inter-defect separation distance. In the late pre-collision regime the symmetry changes within the
cores of defects also become influential. Following the defect collision, in the early post-collision
stage, bulk layer order is approached exponentially in time. At very late times, however, there
seems to be a long-time power-law tail in the order parameter fluctuation relaxation.

I. INTRODUCTION

At low temperatures, almost all materials exhibit phases with broken symmetries. The
low temperature phase is described by an order parameter which exists on some restricted
manifold*D*. Its local position within*D* is then describable in terms of some phase function
Φ. The dynamical processes whereby the symmetries are broken are extremely complicated.
Almost always the order parameter at one place is different from that at another. The
resulting order parameter variation is sometimes relatively strong, but not singular. In this
case the order parameter always remains arbitrarily close to *D*. Defects refer to regions
where the phase function Φ(*−→r*) exhibits singular behavior. They may be points, lines or
surfaces in a bulk system, and it is now known that they may be understood in terms of a
topological classification related to the underlying group structure of the order parameter
manifold [1, 2].

There has long been interest in the physics of defects, long predating the more sophisti-cated topological studies. Not only do the defects induce long-range forces within a structure, but also the bulk material properties of materials filled with defects can be overwhelmingly dominated by the existence of those defects. For example, it is the presence of dislocations [3] which essentially governs the yield stresses, plastic deformations and fracture properties in a solid. Likewise, liquid crystal textures [4], which dominate the visual impact of in-dividual liquid crystal phases, are the product of defect structures in the order parameter configurations. The defect structures are thus only a topologically-mediated indirect effect of the order parameter manifold itself, but this was nevertheless historically sufficient to identify the nature of the phases [5].

Given their essentially topological basis, it is perhaps not surprising that defect structures exhibit much universality. As a result there are often profound mathematical similarities between apparently completely different physical systems, ranging from condensed matter to cosmological structures [6–8]. These similarities are nevertheless not apparent from a naive non-mathematical point of view.

in superconductors and superfluids. Our model line defects are edge dislocations in smectic liquid crystals (LCs) [4].

From a practical point of view, the advantage of studying defects in liquid crystals is that the time-scale of any motions is many orders of magnitude faster than that in solids. Now interesting effects can be observed on reasonable time-scales.

A typical smectic phase consists of a stack of layers, within which there exists liquid-like organization of molecular mass centers [9]. The resulting quasi-two-dimensional system gives rise to logarithmically divergent positional fluctuations with respect to the character-istic sample size. Consequently quasi-long-range positional ordering occurs in finite-sized samples. For all but the mathematical physicist, these systems are one-dimensional solids.

The different smectic phases are classified according to the orientational order within (and between) layers. The simplest phase is the smectic A (SmA) phase. In this, the rod-like molecules tend to be aligned along the layer normal. However, in describing the static and dynamic behavior of edge dislocations in various smectic LC phases the layer ordering plays the dominant role [4, 9], while the other degrees of ordering are only of secondary importance. Thus the relatively simple SmA phase, to which we henceforth restrict our interest, is often sufficient to illuminate the basic mechanisms behind these phenomena.

and Lubensky [15], but the details of the structure have not yet been definitively resolved. Experimental verification is still lacking because of the smallness of the core size. This is typically of the order of a few smectic order parameter correlation lengths. Apart from close to phase transitions this is comparable to a typical molecular size. Edge dislocations can also appear if a change sudden with respect to a relevant smectic ordering relaxation time is imposed on the system. An example is a sudden quench into a smectic phase starting from the isotropic phase.

There have been only a few studies on dynamics of edge dislocations [16–19] in smectics. In these studies the motion of edge dislocations was studied as a function of imposed stress [16–18] and boundary conditions [19]. All these studies employ the classic displacement field description of the smectic ordering, in which order parameter variations are neglected. We shall henceforth refer to this description as the classical model [9, 20].

This theoretical study concerns the mutual annihilation of edge dislocations lying in the same smectic A phase layer. Now order parameter spatial variations play a necessary role, and so the classic displacement field description is insufficient. Note that in the frame of the classical model the edge dislocations in such a configuration do not interact [21].

We shall describe a system in which two line defects are inserted in the same smectic plane. The layer width far from the defects is equal to the equilibrium one. The equi-librium condition is that the layers attain their natural separations everywhere. Obeying topological requirements this state is obtained via annihilation of dislocations. Our problem is to describe the evolution of the starting system, containing the two dislocations, into the equilibrium system, in which they have disappeared.

The study begins with the order parameter configuration at early times. Here there are two well-defined and well-separated dislocations. At intermediate times, however, the proximity of the dislocations affects the order parameter profiles in each of them. Later still the defects collide and annihilate. However, there is still a ghost-like signature of the previous configuration. Finally all non-equilibrium components of the order parameter decay, leaving a uniform planar smectic bookshelf geometry.

appendices.

II. MODEL

Our approach is phenomenological, in that we seek equations of motion for the order parameter. Specifically, we shall use the de Gennes complex order parameter to describe the smectic wave. Although this approach has been questioned in recent years [22, 23], no superior model exists at the moment. We shall use the Landau-de Gennes free energy [11, 13], which we have ourselves used in recent years in a number of studies of inhomogeneous smectic systems [14, 24]. In this initial study of smectic defect dynamics we use the most naive time-dependent Ginzburg-Landau approach. This is equivalent to approaches to nematodynamics which ignore backflow. We believe that this will illuminate the most basic features of the problem. In future work we shall return to the problem and attempt to incorporate backflow properly. We now discuss the specific features of the model in more detail.

A. Order parameter

In the Landau-de Gennes approach[11, 13] the degree of SmA layer ordering is described
by a complex smectic order parameter *ψ* = *ηeiφ*_{. This quantity corresponds to the first}
harmonic term in the Fourier expansion in the spatial variation of the molecular mass density

B. Free energy

The free energy density*f* of the unconstrained SmA phase contains two terms: *fh* and*fe*.
The first term represents the homogeneous contribution to the free energy density, whereas
the second represents the elastic contribution. The free energy *F* of the system is obtained
by integrating *f* over the entire volume of the sample :

*F* =
Z

(*fh*+*fe*)*d*3*−→r .* (1)

For a second order nematic (N) to SmA phase transition the free energy density *fh* can be
expressed as an expansion in *ψ* [11]. To lowest relevant order this is:

*fh* =*α|ψ|*2+

*β*

2 *|ψ|*

4_{,}_{(2)}

where *α* = *αo*(*T* *−TN A*), *αo, β* are positive material constants, *T* is the temperature and

*TN A* the N-SmA phase transition temperature. The minimum of *fh* determines the degree
of bulk smectic ordering: *ηb* =

p

*α*0(*TN A−T*)*/β*. We neglect coupling between the smectic
and nematic order parameters. This can change the order of the smectic-nematic phase
transition, but involves physics which is not central to the present purpose.

The elastic contribution of the free energy density *fe* describes the elastic response to
changes in the smectic ordering. This consists of the nematic (*fe*(n)) and smectic (*fe*(s))
components. It is known that the nematic elasticity interacts with the smectic phase to give
a second gradient squared term in the displacement in the direction parallel to the smectic
layers [13, 21]. The resulting long-range strain field is the solution of a quartic equation.
However, in order to simplify the problem, in this calculation we shall suppose the director

*−*

*→ _{n}*

_{is homogeneously aligned along the direction in which the layers are stacked on average.}

The result of this assumption is that we can neglect the nematic elastic term*fe*(n). Therefore
within our approach only the phase factor field*φ* gives rise to the long-range strain field. In
Appendix I we show that spatial variations in *−→n* give rise only to quantitative changes in
the behavior of our interest.

The smectic elastic term can be expressed as [9, 13, 15]:

These two terms involve positive elastic constants associated with smectic bend (*C⊥*) and

compressibility (*Ck*). The first term tends to align the smectic layer normal along *−→n*.

The smectic compressibility term enforces the layer spacing *d*0. Typically the ratio of the
compressibility to the bend constant is in the region of 1-10 [9]. In our calculation, for
simplicity, we shall take this ratio to be unity and set*C⊥* =*Ck* *≡C*. The changes introduced

by*C⊥* *6*=*Ck* are analyzed in Appendix I.

We now identify the important characteristic lengths that enter our study [9]. These are:

(a) the smectic layer separation *d*0;

(b) the separation distance *L* between defects;

(c) the smectic order parameter correlation lengths*ξk* =

µ

*Ck*

2*|α|*

¶_{1/2}

and*ξ⊥* =

µ

*C⊥*

2*|α|*

¶_{1/2}
.

The quantities *ξk* and*ξ⊥*measure the response of the system to locally induced

perturba-tions in the smectic ordering in the direcperturba-tions respectively along the smectic layer (*ξk*) and

perpendicular to it (*ξ⊥*). In our calculations, the equality of the elastic coefficients implies

that the correlation lengths are also equal, and we set *ξ⊥* = *ξk* *≡* *ξ*. Furthermore, so long

as order parameter variations can be neglected, as we show in the Appendix II, the
Euler-Lagrange equation for the variation of the phase factor*φ* alone is scale-free. As a result the
variations in *φ* adapt only to the constraints imposed by the geometry of the problem.

C. Dynamics

We adopt the time-dependent Ginzburg-Landau model, in which

*γ∂ψ*
*∂t* =*−*

*δf*

*δψ∗,* (4)

has been made by Bruinsma and Safinya [26] and by Brand et al [27]. In the absence of a full and reliable dynamical theory, we restrict the study to order parameter relaxation. We note that in the case of nematic liquid crystals, the effect of ignoring backflow (i.e. hydrodynamic coupling) can in some cases simply change the effective viscosity constant. However in some specific ranges qualitative changes can take place that are not considered in our study [28, 29]. An attempt taking into account a flow into the model is demonstrated in Appendix I.

We may remark that this approach is equivalent to making an ansatz for the dissipation
function *D*, and supposing that the free energy gained per unit time is entirely dissipated.
Accordingly *−dF*

*dt* =*D*, where *D*=

Z

*gd*3*−→ _{r}*

_{. The full theory would include inertial effects}as well as a more sophisticated formulation of the dissipation function. The simple TDGL dissipation function takes the form:

*g* =*γ*

¯
¯
¯
¯*∂ψ _{∂t}*

¯ ¯ ¯ ¯ 2

*,* (5)

where *γ* is an effective smectic drag viscosity.

It is now possible to make some initial observations based on dimensional analysis. The
characteristic order parameter relaxation time is roughly given by *τ* *∼* *γ*

*|α|* and is thus

proportional to the square of the smectic order parameter correlation length. By contrast,
there is also a time*τφ*characterizing distortions in the smectic phase*φ*. This depends on the
typical linear size *Ld* of an imposed distortion. We find that *τφ∼*

*γL*2
*d*

*C* , where *C* stands for

an appropriate smectic elastic constant. We develop this argument further in the Appendix II.

D. Geometry of the problem

The geometry of the problem is depicted in Fig.1. The smectic layers are stacked along the

the solutions. Thus we do not expect spatial variations along the *y*-axis, implying that

*ψ*(*−→r*) =*ψ*(*x, z*).

The problem has further reflection symmetry in the*x*= 0 and*z* = 0 axes. This symmetry
permits us to restrict the calculation to a single quadrant, and we choose the quadrant

*x <* 0*, z >* 0. The region over which calculations are actually carried out is shown in Fig.
1 and is surrounded by bold lines. Only one of the two defects remains in our calculation
domain; the behavior of the other can be inferred by reflection symmetry.

We note that the symmetry conditions at the reflection planes *x* = 0 and *z* = 0 are
different. Reflection in the *z* = 0 plane leads to the condition *ψ*(*x, z*) = *ψ∗*_{(}_{x,}_{−}_{z}_{). This}

is equivalent to the condition *u*(*x, z*) = *−u*(*x,−z*), where *u*(*x, z*) is the displacement of a
smectic layer from its equilibrium position. By contrast, reflection in the *x*= 0 plane yields
the condition *ψ*(*x, z*) =*ψ*(*−x, z*); this is equivalent to the condition *u*(*x, z*) = *u*(*−x, z*).

These symmetry relations govern the boundary conditions at the walls of the calculation
domain. This domain is cuboid with sides*Lx, Ly, Lz*. Because of the translational symmetry
in the *y*-direction, out of these, only the quantity *Ly* enters the non-dimensionalization.

E. Parameterizations and equations

We use the following non-dimensionalizations:

(a) The scaled smectic order parameter *η*e=*η/ηb*;

(b) The dimensionless energy *F*e=*F/F*0, where *F*0 =*Cηb*2*Ly*;

(c) Lengths are measured in terms of the smectic order parameter correlation length e*x*=

*x/ξ*, e*z* =*z/ξ*,*L*e=*L/ξ*, *q*e0 =*q*0*ξ* etc.;

(d) Time is measured in units of the smectic order parameter relaxation time: e*t*=*t/τ*.

The scaled order parameter can be expressed as

e

*ψ* =*ηe*e *iφ*=*ηe*e *i(q*0(z*−u))* _{= Ψ}* _{e}iq*0

*z*

in Ψ = ˜*η*exp(*−iq*0*u*(*x, z*)). However, in order to circumvent problems with the definition of
the phase *φ* where the order parameter is small inside the defect cores, we represent Ψ in
terms of its real and imaginary components: Ψ = *ηe*e *−iq*0*u* = *A*+*iB* [10, 24]. In all further

calculations we drop all the tildes.

The quantity Ψ is a normalized order parameter which includes the degree of order and departures from perfect smectic order. The free energy can now be rewritten in terms Ψ. The explicit effect of the smectic wave is lost and the theory reduces to the well-known gradient theory with a complex order parameter. The free energy is now

*fh* =
1
2

µ

*−|*Ψ*|*2_{+}1
2*|*Ψ*|*

4 ¶

*,* (6)

*fe* = *|∇*Ψ*|*2*.* (7)

The time evolution equation (4) can now be written as

*∂*Ψ

*∂t* = 2*∇*

2_{Ψ + Ψ}¡_{1}_{− |}_{Ψ}* _{|}*2¢

_{.}_{(8)}

In terms of the parameters *A*(*x, z, t*)*, B*(*x, z, t*), the dynamical Euler-Lagrange equations
can be written as:

1 2

*∂A*
*∂t* =

*∂*2_{A}

*∂x*2 +

*∂*2_{A}

*∂z*2 +
1
2*A*

¡

1*−*(*A*2+*B*2)¢*,* (9)

1 2

*∂B*
*∂t* =

*∂*2_{B}

*∂x*2 +

*∂*2_{B}

*∂z*2 +
1
2*B*

¡

1*−*(*B*2_{+}* _{A}*2

_{)}¢

_{.}_{(10)}

F. Boundary and initial conditions

The problem is parabolic in time and ellipsoidal in space. We need to specify initial values
Ψ(*x, z,*0), as well as boundary conditions on the surfaces *z* = 0, *x* = 0, *z* = *Lz*, *x* = *−Lx*.
We use the following boundary conditions:

(a) *z* = 0. Here the symmetry relation *u*(*x, z*) = *−u*(*x,−z*) *⇒* *u*(*x,*0) = *−u*(*x,*0) = 0,
i.e.:

*∂A*

(b) *x*= 0 : Here the symmetry relation is *u*(*x, z*) = *u*(*−x, z*). Now the condition is that

*∂A*
*∂x* = 0;

*∂B*
*∂x* = 0*.*

(c) *z* = *Lz* : There is no symmetry relation, and so we simply suppose that a stable
situation has been reached sufficiently far from the defects. This implies that the
gradients perpendicular to the wall are zero, or

*∂A*
*∂z* = 0;

*∂B*
*∂z* = 0*.*

(d) *x*=*−Lx* : This is analogous to the previous case:

*∂A*
*∂x* = 0;

*∂B*
*∂x* = 0*.*

We observe, however, that whereas conditions (a), (b) are set by symmetry, conditions (c) and (d) are set by convenience, and approximate the situation as the distance from the defects approaches infinity. If other plausible conditions are applied on the latter boundaries (e.g. we suppose that they approximate to undisturbed smectic layers) negligible difference in our results is observed.

We use the following initial ansatz for the amplitude and phase of smectic complex order
parameter. At the centre of the defect we set *η* = 0. We vary the ordering linearly with
the distance from the defect centre, reaching the bulk value *ηb* at the distance equal to the
smectic order parameter correlation length. Elsewhere we set*η* =*ηb*. For the phase shift we
set *φ*= *π−ϕ*, where *ϕ*=*ArcT an*

³
*z−zd*

*x−xd*

´

and the defect is placed at (*x, z*) = (*xd, zd* = 0).
This ansatz for the phase shift corresponds to no displacement of layers on the left of the
defect and to the half-layer displacement to the right of it. Then the corresponding *A*(*x, z*)
and *B*(*x, z*) profiles are calculated using Eqs.(9,10). Quasi-equilibrium profiles for relatively
large separations*L*of defects are obtained at a short time relatively to the annihilation time.
We also used other initial ansatz for smectic layer displacement [21]. All ansatz profiles have
retraced into the same solution after a time period equal to a few correlation times *τ.*

III. RESULTS

(i) After a relatively short time, of the order of a few relaxation times, the local core structure reaches the quasi equilibrium order parameter profile.

(ii) From this time on we monitor the annihilation dynamics. In the *pre-collision regime*
well-distinguished defects approach each other to reduce the effective layer curvature
of the system. The defects attract because in the absence of the defects the elastic
energy is reduced. If the defects approach each other, sufficiently far away, the two
defects essentially cancel each other out. If the defects are separated by a distance *L*,
the critical distance over which the defects no longer give rise to a displacement field
is of the order of *L*. The smaller the separation, the smaller the elastic energy.

(iii) The defects then*collide. In the collision the defects merge and it is no longer possible*
to distinguish two separate entities.

(iv) In the *post-collision* regime the disturbed structure resulting from the defect collision
gradually decays into a bulk, undistorted state.

We are able further to distinguish in each of the pre- and post- collision regimes two
different time regimes, resulting from the different characteristic time scales for *η*and *φ*. In
what follows we analyze in more detail the different stages in the annihilation process.

Some characteristic stages of the annihilation dynamics are shown in Figs. 2 and 3. On
the left panel we show the layer profiles with superimposed smectic order parameter contour
plots. The contours label the values*η/ηb* = 0*.*95 (the most outer one)*, η/ηb* = 0*.*8*,*0*.*6*,*0*.*4*,*0*.*2
and *η/ηb* = 0*.*05 (the most inner one). On the right panel the spatial variation of the order
parameter along the *x*-axis is shown at *z* = 0 (the most bottom curve), *z* =*ξ,*2*ξ,*3*ξ,*4*ξ,*5*ξ*

and *z* = 6*ξ* (the most upper curve).

is due to the equal elastic constant approximation (*ξ⊥* =*ξk*). For a real elastic anisotropy,

where *ξk* *> ξ⊥*, the core is extended in the *z* direction.

With time the defects gradually enter the *late pre-collision regime,* shown in Figs.3a.
Now the defect core structure of a defect seems to be influenced by the interaction with its
neighbor. The order parameter profiles in the cores gradually lose their cylindrical shape and
become extended in the direction joining the defects. The inner contours remain cylindrical,
but some outer contours in Figs.3a are now pear-shaped, and the very outermost contours
even encircle both defects. As the defects further approach, these features become more
pronounced, and the departures from a cylindrical shape begin closer and closer to the defect
centers, by which we mean the points at which the layering order parameter disappears.
Eventually the defect core structures significantly overlap and it is no longer possible to
distinguish one from another. Detailed examination of Figs.3a also shows that the time
evolution of the outer contours is delayed with respect to those near the defect centers. This
is probably the result of a relatively slow layer readjustment which follows from a phase
relaxation time-scale*τφ∼γL*2*/C*. We discuss this point further in the Appendix II.

In the*collision, shown Fig.3b, the melted regions of both defects merge. After this event*
the ”nonsingular” *early post-collision stage* is entered. This stage is characterized by the
apparent growth of the order parameter at the collision site on a time scale given by *τ*.
This feature is shown in Fig.3c. Gradually the quasi-equilibrium order parameter profile
is established, adiabatically adjusting to the slower layer displacement dynamics. During
this period the degree of layering approaches that expected in an equilibrium smectic phase.
Finally, the *late-post-collision stage* is essentially characterized by the layer displacement
dynamics, by which the exact thermodynamic equilibrium is asymptotically approached.
During this period, the layer displacements disappear.

We find that *L*(*t*) is rather close to a power law dependence *L* *∝* (*tc−t*)*λ*, where the
*collision time* *tc* is the time taken until the defects mutually annihilate. The exponent

*λ* *≈* 0*.*5*±*0*.*05. However, there are small departures from this rule, and the best fitted
exponent seems to depend monotonically on the total system size. The value for *λ* quoted
above is an extrapolation to infinite system size. We shall return to the departure from the
exact scaling law in the next section.

An initial size-annihilation time dependence law *L*(*t*) can be inverted to yield a law for
the defect approach velocity*v*(*L*). The power law relation *L∝*(*tc−t*)*λ* implies an analogous
power law relation *v* *∝* *L*1*−*1/λ_{. Taking the extrapolated} _{λ}_{= 0}_{.}_{5 suggests the relationship}

*v* *∝* *L−*1_{. In Fig.4b we make a loglog plot of the} _{v}_{(}_{L}_{) dependence. One observes a slight}
change in the behavior when*L*(*t*)*∼ξ*). This is unsurprising, given that structural variations
in*η* near the defects centers become significant.

The asymmetry of the core in this regime is depicted in Fig.5. One sees that the core
size along the *z* direction remains approximately unaffected and gradually increases in the

*x* direction on approaching*tc*. In the mean time the size in the *z*-direction slightly shrinks,
revealing the tendency to conserve the amount of the melted region.

An illustrative representation of the characteristic *η*(*t*) variation is shown in Fig.6. We
plot the time evolution of the order parameter in the middle of the plane through both
defects, i.e. *ηm* = *η*(*x* = 0*, z* = 0). For *L >* 10*ξ* it holds *ηm* *∼* 1. At later distances (i.e.
times) *ηm*(*t*) monotonically decreases indicating the merging of the cores of defects. Just
before and after the collision the linear dependence *ηm* *∝ |t−tc|*is observed. This behavior
also emerges from the approximate solution Eq.(11). In it we follow the value of *η* at the
mirror plate at *t < tc* and get *ηm* *∝tc−t.*

After the collision *ηm* asymptotically approaches its bulk thermodynamic value *ηb*. In
the late pre-collision regime the numerical calculations indicate *ηb−ηm* *∝*1*/*(*t−tc*). This
suggests adiabatic adjusting of *ηb* to the much slower Φ time evolution.

IV. DISCUSSION

We first discuss the *L*(*t*) *∼* (*tc−t*)1/2 law, which as we have seen above is equivalent
to a *v*(*L*)*∼* *L−*1_{. We derive a simple ansatz, using Eqs.(9,10), which gives insight into the}

*L*∝*√tc−t*dependence. We concentrate on the behavior of *A*(*x, t*) at a defect site. Exactly
at the defect origin *A*= 0. For*φ*= 0, *A*=*η, B* = 0; and *η*= 0 at the defect center, but the
derivatives of *A* and *B* have finite values. Exactly at the defect center, neglecting spatial
variations in the z direction, (in scaled units) eq.(9) reduces to *∂A*

*∂t* *∼*
*∂*2_{A}

*∂x*2.
A possible solution to this equation is:

*A*=*c*(*−*(*tc−t*) +*x*2*/*2)*,* (11)
where *c* is a constant. The defect position is given by the implicit equation *A*(*x, t*) = 0.
Combining this with eq.(11) yields:

*x*=p2(*tc−t*)*,* (12)

which, as shown in Fig.4a, describes the whole pre-collision regime rather well.

It is possible to estimate the experimental time scale corresponding to the cases we have
studied. We rewrite eq.(12) in its dimensional form: *x*2 _{= 2}*ξ*2

*τ* (*tc−t*)*≡* 2*D*(*tc−t*), where
*D* plays the role of a diffusion constant. For *D* *∼* 10*−*12* _{m}*2

*1*

_{s}−_{[18] and}

_{ξ}_{of the order of}nm (which holds true well into the SmA phase), we obtain

*τ*

*∼*10

*−*6

_{s}_{. With this in mind,}the longest calculations in Fig.4a extend over a time scale of 10

*−*4

_{s}_{. However, our approach}is also applicable close to the N-SmA phase transition, where the dynamics is considerably slower. In this regime our calculations may correspond to longer experimentally accessible time scales.

Similar behavior is observed in annihilation of orientational line defects in the nematic
and smectic C phases [30–38]. The role of *η* and *φ* is in this case played by nematic
or-der parameter and nematic director field, respectively. All these studies, with exception of
Ref.[38], concentrate on the pre-collision regime. These theoretical, experimental and
simu-lation studies confirm the basic *L∝√t−tc*, i.e. *v* *∝*1*/L* behavior. We note that for point
defects the balance of forces is different, and in general the *v* *∼L−*1 _{law no longer obtains.}

model system is described by the free energy *F* =
Z

*K|∇φ|*2*dV*. Here *K* stands for a
representative elastic constant of the LC phase and *φ* is the relevant order parameter field
(e.g. the phase factor in a smectic phase a representative angle of the nematic director field in
the nematic phase). The kinetics of the system is governed by the dissipation relaxation law

*−dF*

*dt* = *D*, where the dissipation function is given by *D* =*γ*

Z ¯¯
¯
¯*∂φ _{∂t}*

¯ ¯ ¯ ¯ 2

*dV*. The interacting
pair of defects are placed along the *x*-axis, separated by a distance *L*. Then the defect
structure survives over a distance of the order of *L* in all directions, and is quenched on
length scales than this. Then

*∂φ*
*∂t* *∼*

*∂φ*

*∂xv*; (13)

The dissipation function and the energy function will have the same dependence on
separa-tion *L*, because they are both gradient functions. Let this be *G*(*L*). Then

*G*(*L*)*v*2 _{∼}*d*

*dtG*(*L*)*∼*
*dG*

*dLv,* (14)

yielding

*v* *∼* *d*ln*G*

*dL* (15)

between defects. If *G*(*L*) is power law or logarithmic, we obtain *v* *∼* 1

*L.*

Some authors [30–32, 34] have derived logarithmic corrections to the basic *v*(*L*) law.
In general these studies have considered an orientational order parameter, but their
con-siderations probably apply to the present study. Pargellis *et. al.* suggested *tc* *−* *t* =

*CL*2_{(}_{Log}_{(}_{L/R}

*c*) *−*0*.*5), which is equivalent to *v*(*L*) *∼* (*L*ln*L*)*−*1. Here *C* is a constant
and*Rc*is proportional to the core size of a defect. We do find a better fit to our*L*(*t*) results
in the early pre-collision regime with this ansatz, but it requires *Rc* *<< ξ*. The significance
of this result is unclear.

Under these circumstances close analogy between our results and studies of disclination annihilation might well be expected, although naturally some differences would also occur because of the different order parameter symmetries. The index 1/2 nematic disclination and the index 1 XY disclination are each minimal from a topological point of view. In the orientational picture the positive and negative index defects are not identical, and thus a breaking of the mirror symmetry in principle is not only possible but expected. However, the mapping of the XY model onto a smectic in some sense forces both positive and negative index disclinations to map onto identical dislocations but with opposite Burgers vector, thus restoring the mirror symmetry.

The dynamics of our model is governed by one effective viscosity constant *γ* introduced
by the dissipation term in Eq.(5). This term takes into account only dissipation related to
the time changes in the SmA order parameter. It introduces two characteristic time scales

*τ* and *τφ* (see Appendix II) that are related to the translational order parameter *η* and the
phase factor *φ* dynamic behavior, respectively. In order to understand microscopic origins
of *γ* we relate the Ginzburg-Landau (GL) model that we use with the classical (CL) model.
For the latter model the link with experimental parameters is relatively well established.
We originate from Eq.(4), the time dependent Ginzburg-Landau equation *γ∂ψ _{∂t}* =

*−*,

_{δψ}δf∗describing local changes of the order parameter *ψ* =*ηeiφ*_{. To take into account flow effects}
we replace the partial time derivative in Eq.(4) with the material derivative. We get *γdψ _{dt}* =

*γ*¡*∂ψ _{∂t}* +

*v· ∇ψ*¢=

*−*, where

_{δψ}δf∗*−→v*represents the velocity of the material flow. The CL form

of this equation is obtained in the ”phase approximation”, where spatial variations in *η* are
neglected. We further introduce the displacement field in a ”classical way” as*φ* =*q*0(*z−u*)
and neglect the nonlinear term *v* *· ∇ψ*. The equation *vz* *−* *∂u _{∂t}* =

*−λpδf*follows, that is commonly used to study the dynamics of the displacement field. The quantity

_{δu}*λp*= 1

*/*(

*γq*20) is known as the permeation constant. The permeation refers to the motion of fluid through the layers. Close to the N-SmA phase transition the permeation is particularly easy and

*λp* ∝ 1*/*(*TN A* *−T*). Deep in the SmA phase it holds *λp* *∼* *d*20*/η⊥*. Here *η⊥* describes a

fluid viscosity constant along the smectic layer normal. For *T << TN A* the permeation
flow typical length is given by *lp* *∼*

p

*ηvλp* *∼*
p

*ηv/η⊥d*0, where *ηv* stands for a typical
viscous constant. In order to calculate the velocity field [16] the Navier-Stokes equation
(in it *δf*

In our approach we neglect the velocity field. If the diffusion within smectic layers, where liquid-like behavior is expected, is an infinitely fast process, only the permeation controls the motion of edge dislocations. But if diffusion can not relax immediately the vacancies created by permeation also the viscosity within smectic layers is important.

We also believe that the material flow plays weaker role in the annihilation of smectic edge dislocations in comparison to the annihilation of nematic defects. In the latter case the flow is important and is the main reason behind asymmetric annihilation process (i.e. the defects with a positive Frank index are faster) of defects. When the nematic defect approach each other, the reorientation of molecules takes place, that is relatively strongly coupled with the fluid flow. In the absence of flow the main source of dissipation is the region surrounding the defects. If the flow is triggered the dissipation is delocalized through the region in which the flow is present. On contrary the annihilation process of edge dislocations does not require reorientation of LC molecules, therefore the coupling with the flow is weaker. In addition the flow would disrupt smectic layers what is relatively energetically costly, particularly deep in the SmA phase.

It is possible that our simulation does not appropriately recover events close to the
colli-sion of defects, where the relative velocity of defect is very high. The important parameter
measuring the credibility of our approach is the so called Deborah number [29] *De*, defined
as*De* =*rτ*. Here*r*stands for the shear rate and*τ* is the relevant order parameter relaxation
time. If *De* *<<* 1 then the role of hydrodynamics effects is expected to be negligible. We
proceed by estimating the critical velocity *vc* for which our calculations are not reliable by
requirement *De* = 1*.* We set *r* *∼* *∂v _{∂z}x* and

*τ*is the translational order parameter relaxation time. The shear rate is the largest close to defects. If we set that the velocity field drops to zero over

*Nd*layers, we get the condition

_{N}v_{d}c_{d}_{0}

*τ*= 1. For

*τ*

*∼*10

*−*6

*s*,

*d*0

*∼*3

*nm*and

*Nd*= 3 we get

*vc*

*∼*1

*cm/s*. This value of velocity is very high. Typically edge dislocations move with the velocity

*v <*10

*−*2

_{cm/s}_{[18].}

conventional smectic phase a climb of a dislocation is much easier than a glide because a glide
necessitates layer breaking. Therefore a relevant characteristic time scale in a layer plane
direction and perpendicular to it are expected to be apparently different. The classical
theory [4] predicts that the interaction force in the x-direction between dislocations can
become repulsive for ∆*z* *6*= 0 for a sufficiently small separation *L*. Therefore for the case
that gliding is apparently less probable than climbing a pair of edge dislocations is expected
to get caught in a metastable state at a separation *L* = *L*(∆*z*). The system would then
remain in this state until a fluctuation triggers a gliding event enabling annihilation into
the defectless state. In order to simulate this case with our model an anisotropic symmetry
allowed dissipation term (see Eq.(5)) including different viscosities in a layer plane and
perpendicular to it should be introduced, which is the focus of our future work.

V. CONCLUSION

We have studied the annihilation of edge dislocations in the bulk SmA phase using the
phenomenological Landau-Ginzburg approach. We have begun with a pair of facing edge
dislocations at a distance *L*0 *>> ξ*. Within the classical approach such dislocations would
not interact. In our approach the interaction is enabled by the smectic bend elastic free
energy term, weigthed by the elastic constant *C⊥*.

has two qualitatively different stages. In the early post-collision regime the order parameter
profile at the collision site exponentially (with characteristic time *∼* 1*.*5*τ*) approaches the
quasi equilibrium *η*(*−→r*) profile, fingerprinting the momentary *φ*(*−→r* ) pattern. In the late
post-collision regime the equilibrium profile is approached as *ηb−η∝*1*/*(*t−tc*).

Most of our calculations were carried out for the isotropic XY limit, where the dynamics
of the system is described solley by the complex order parameter*ψ*. However we have shown
that deviations from this approach in general give rise to relatively small quantitative changes
in the behavior of our interest.

Acknowledgments

This research was supported by a ESF network project COSLAB and Slovenian Office of Science.

Appendix I: Deviations from the isotropic XY-behavior

In this appendix we estimate how the i) nematic director field variations, ii) smectic elastic anisotropy and iii) the flow influence the results obtained in the main part of the article.

We first study cases i) and ii). We parametrize the director field as *−→n* = (sin*θ,*0*,*cos*θ*),
where *θ* = *θ*(*x, z*). For sake of simplicity we restrict *−→n* to vary in the (*x, z*) plane. In the
single Frank nematic elastic constant approximation the nematic elastic free energy
contri-bution is given by *fe*(n) = *K*_{2}

³¡_{∂θ}*∂x*

¢_{2}
+¡*∂θ*

*∂z*
¢_{2}´

, where *K* is the representative Frank nematic
elastic constant. The dissipation function of the system (see Eq.(5)) is approximately
ex-pressed as*g* =*γ*(s)¯¯*∂ψ*

*∂t*
¯
¯2

+*γ*(n)¡*∂θ*
*∂t*

¢_{2}

, where*γ*(s)_{and}* _{γ}*(n)

_{approximate the viscosity properties}in the smectic and nematic degrees of freedom, respectively. We use the parametrization given is Subsection.II.e, measure all distances in units

*ξ⊥*, and we get

1 2

*∂A*

*∂t* = *cxx*
*∂*2_{A}

*∂x*2 +*czz*

*∂*2_{A}

*∂z*2 +*εcxz*

*∂*2_{A}

*∂x∂z* +*εcx*
*∂A*
*∂x* +*εcz*

*∂A*

*∂z* +*cA,* (16)

1 2

*∂B*

*∂t* = *cxx*
*∂*2_{B}

*∂x*2 +*czz*

*∂*2_{B}

*∂z*2 +*εcxz*

*∂*2_{B}

*∂x∂z* +*εcx*
*∂B*

*∂x* +*εcz*
*∂B*

*∂z* +*cB,* (17)

1 2

*∂θ*

*∂t* = *κn*

µ

*∂*2_{θ}

*∂x*2 +

*∂*2_{θ}

*∂z*2
¶

+ *cθ*

*κτ*

Here

*ε* = *Ck*

*C⊥*

*−*1*, κn*=

*γ*(s)_{K}

*γ*(n)_{C}

*⊥ηb*2

*, κτ* =

*γ*(n)

*γ*(s)*, cxx* = 1 +*ε*sin
2_{θ, c}

*zz* = 1 +*ε*cos2*θ,*

*cxz* = sin (2*θ*)*, cx*=

*∂θ*

*∂x*sin (2*θ*) +
*∂θ*

*∂z* cos (2*θ*)*, cz* =
*∂θ*

*∂x*cos (2*θ*)*−*
*∂θ*

*∂z* sin (2*θ*)*,*
*cA* = *q*0*B*

*∂θ*

*∂x*((1 +*ε*) cos*θ−ε*cos(2*θ*)) +*q*0*B*
*∂θ*

*∂z* (*−*(1 +*ε*) sin*θ*+*ε*sin(2*θ*)) +
*q*0

*∂B*

*∂x* (2(1 +*ε*) sin*θ−ε*sin(2*θ*)) + 2*q*0
*∂B*

*∂z*

¡

(1 +*ε*) cos*θ−ε*cos2_{θ}_{−}_{1}¢_{+}
1

2*A*
¡

1*−*(*A*2_{+}* _{B}*2

_{)}¢

*2 0 ¡*

_{−}_{Aq}(*ε*+ 1)(1*−*cos*θ*)2_{+ sin}2* _{θ}*¢

_{,}*cB* = *q*0*A*

*∂θ*

*∂x*(*−*(1 +*ε*) cos*θ*+*ε*cos(2*θ*)) +*q*0*A*
*∂θ*

*∂z* ((1 +*ε*) sin*θ−ε*sin(2*θ*)) +
*q*0

*∂A*

*∂x* (*−*2(1 +*ε*) sin*θ*+*ε*sin(2*θ*)) + 2*q*0
*∂A*

*∂z*

¡

*−*(1 +*ε*) cos*θ*+*ε*cos2_{θ}_{+ 1}¢_{+}
1

2*B*
¡

1*−*(*A*2_{+}* _{B}*2

_{)}¢

*2 0 ¡*

_{−}_{Bq}(*ε*+ 1)(1*−*cos*θ*)2_{+ sin}2* _{θ}*¢

_{,}*cθ* = *εcθ1*+ (1 +*ε*)*cθ2,*

*cθ1* =
Ãµ
*∂A*
*∂z*
¶_{2}
*−*
µ
*∂A*
*∂x*
¶_{2}
+
µ
*∂B*
*∂z*
¶_{2}
*−*
µ
*∂B*
*∂x*
¶_{2}
+ 2*q*0

µ

*A∂B*
*∂z* *−B*

*∂A*
*∂z*

¶

+*q*2_{0}¡*A*2+*B*2¢

!

sin(2*θ*) +

2
µ
*−∂A*
*∂x*
*∂A*
*∂z* *−*
*∂B*
*∂x*
*∂B*

*∂z* +*q*0

µ

*B∂A*
*∂x* *−A*

*∂B*
*∂x*

¶¶

cos(2*θ*)*,*

*cθ2* = 2
µ

*q*0
µ

*B∂A*
*∂z* *−A*

*∂B*
*∂z*

¶

*−q*2
0

¡

*A*2_{+}* _{B}*2¢
¶

sin*θ*+ 2*q*0
µ

*A∂B*
*∂x* *−B*

*∂A*
*∂x*

¶
cos*θ.*

The dynamics exhibits only relatively small quantitative changes if the nematic distortions
or the anisotropy of smectic elastic constants are allowed. This can be inferred from Fig.7
where we compare the *L*(*t*) dependencies for a) *Ck*

*C⊥* = 1, *κn* = *∞*, b)

*Ck*

*C⊥* = 5, *κn* = *∞*,

and c) *Ck*

*C⊥* = 1, *κn* = 0. In the limit *κn* = *∞* the nematic director field is strictly aligned

along the *z*-coordinate. For *κn* = 0 the smectic elastic constants dominate the behavior
of *−→n*. Therefore *−→n* is forced to be aligned along the smectic layer normal if *η >* 0. For
conventional LCs one expects *κn∼*10. Note that for *κn*= 1 the characteristic times for the
nematic director and smectc phase factor variations are comparable. The case a) is treated
in the main part of the article. Comparison of cases a) and c) reveals the magnitude of
variations in the*L*=*L*(*t*) dependence if *−→n* variation is allowed within the model. Note that
the time in Fig.7 is set to zero at the start of simulation.

smectic layer normal. In the limit *κn* = 0, where maximal deviations of the director field
take place, we get for the maximal tilt angle *θ*max*∼*300. For *κn* = 10 we get *θ*max*∼*30.

We also find that the dynamics in the post-collision regime in negligible influenced for described variations.

We have also checked the change of shape of smectic order parameter contour plots
encircling an isolated edge dislocation as the ratio *Ck/C⊥* is varied. Circular contours in

the case of equal smectic constants are deformed into elliptical ones for *Ck/C⊥* *>* 1. For

*Ck/C⊥* = 5, the ratio between longest and shortest diameter of the ellipsis roughly equals

to two, in line with the scaling prediction *ξk/ξ⊥* =

p

*Ck/C⊥* =

*√*

5*∼*2*.*2.

We next estimate the influence of hydrodynamic flow on *L*=*L*(*t*). For simplicity we set

*Ck/C⊥* = 1 and*−→n* = (0*,*0*,*1). The influence of hydrodynamics can be roughly estimated by

including advection terms in dynamical equations for*A* and*B*. For this purpose we replace
partial time derivatives in dynamical equations with total derivatives. For example in Eq.(8)
we introduce the replacement *∂ψ _{∂t}*

*→*

*dψ*=

_{dt}*∂ψ*+ (

_{∂t}*−→v*

*· ∇*)

*ψ*, where

*−→v*is the mass flow velocity and

*∇*stands for the gradient operator.

We consider the case that is schematically shown in Fig.1, focusing on the defect to the
left. The defect is moving to the right pushing forward the molecules in front of it. These
molecules initially constitute the ”inserted” layer that gives rise to the pair of defects. In the
mean time the molecules from the neighboring layer above (below) the inserted layer move
downwards (upwards) to fill the established empty space. Therefore, when a molecule in
the inserted layer just in front of the defect moves for a distance *a⊥* to the right, the nearby

molecules in the surrounding layers move in the vertical direction for a distance *ak/*2. Here

*a⊥* and*ak* estimate the width and length of a rodlike LC molecule, respectively. If the fluid

is incompressible then the velocity field at the defect origin can be approximatelly expressed
as *−→v* = *vd*(1*,*0*,*_{2a}*ak _{⊥}*). Here

*vd*describes the velocity of the defect. We further assume that the velocity field decays towards zero linearly with the distance

*ρ*=p(

*x−xd*)2+ (

*z−zd*)2 from the defect origin. The velocity is set to zero for

*ρ≥ξ*. In order to estimate the maximal influence of the advection term we set (

*−→v*

*· ∇*)

*ψi*=

*vd*

³

1*−* *ρ _{ξ}*´ ³¯¯

*dψi*

*dx*
¯
¯_{+} *ak*

2a*⊥*

¯
¯*dψi*

*dz*
¯

¯´ _{for} _{ρ < ξ}

Appendix II: Typical relaxation times

We analyze typical relaxation times of a slightly distorted smectic A phase. We assume
that the layers are stacked along the z-axis and *−→n* = (0*,*0*,*1). The smectic order parameter
is parameterized as *ψ* =*ηeiφ*_{.}

We first consider variations in *η* and set *φ* = *q*0*z*. We expand *η* = *ηb* +*δη* about its
equilibrium value *ηb* =

p

*−α/β* up to quadratic term in*δη*. With this in mind one gets

*f* *∼* *fb*(*ηb*) + 2*|α|δη*2+*C|∇δη|*2*,* (19)

*g* *∼* *γ*

µ

*∂δη*
*∂t*

¶_{2}

*.* (20)

The static Euler-Lagrange equation reads *C∇*2_{δη}_{= 2}_{|}_{α}_{|}_{δη}_{, defining a typical relaxation}
distance*ξ* =

s

*C*

2*|α|*.

Neglecting spatial variations the dynamic equation yields 2*|α|δη* = *−γ∂δη*

*∂t* , defining

the relaxation time *τ* = *γ*
2*|α|* *∼*

*γ*

*|α|*. Note that taking into account spatial derivatives

in *δη* affects the dynamics only quantitatively. For example, let us take into account in

Eq.(A1) spatial variations along the x-axis. In typical cases the contribution *C*

µ
*∂δη*
*∂x*
¶_{2}
*∼*
*C*
µ
*δη*
*ξ*
¶_{2}

*∼*2*|α|δη*2 _{renormalizes the second term in Eq.(}_{II.}_{1), leading to} _{τ}_{∼}*γ*
4*|α|*.

In analyzing the response of the phase factor *φ* we assume spatially homogeneous profile

*η*(*−→r*) = *ηb*. Consequently we get

*f*(s)

*e* = *Cη*2
Ãµ
*∂φ*
*∂x*
¶_{2}
+
µ
*∂φ*
*∂y*
¶_{2}
+
µ
*∂φ*
*∂z* *−q*0

¶_{2}!

*,* (21)

*g* = *γη*2
µ

*∂φ*
*∂t*

¶_{2}

*.* (22)

The static Euler-Lagrange equation is now *∇*2*φ*= 0, which does not introduce any scale
into the system. Therefore the variations in *φ* typically adjust to the constraints imposed
by boundary conditions.

Let us assume that *φ* evolves over the distance *Ld*, therefore *fe*(s) *∼* *Cη*2
µ

*φ*
*Ld*

dynamic equation reads *Cφ*

*L*2
*d*

=*−γ∂φ*

*∂t*, defining the time scale *τφ∼*
*γL*2

*d*

*C* *.*

[1] L. Michel, Rev. Mod. Phys.52, 617 (1980).

[2] H.-R. Trebin, Adv. Phys.31, 195 (1982).

[3] V. Volterra, Rendiconti della R. Academia dei Lincei, serie 5 14, 351 (1905).

[4] M. Kleman, *Points, Lines and Walls* (John Wiley, Chichester., 1983).

[5] G. Friedel, Annales de Physique 18, 273 (1922).

[6] N. D. Mermin, Rev. Mod. Phys. 51, 591 (1976).

[7] M. V. Kurik and O. D. Lavrentovich, Sov. Phys. Uspekhi. 31, 196 (1988), [Usp. Fiz. Nauk

154, 381 (1988)], and references therein.

[8] Http://theory.ic.ac.uk/coslab.

[9] P.-G. de Gennes and J. Prost,*The Physics of Liquid Crystals*(Oxford University Press, Oxford

U.K., 1993).

[10] M. Slavinec, S. Kralj, S. ˇZumer, and T. J. Sluckin, Phys.Rev. E63, 031705 (2001).

[11] P.-G. de Gennes, Solid State Commun. 10, 753 (1972).

[12] A. A. Abrikosov, Zh. Eksp. Teor. Fiz. 32, 1442 (1957), [Sov.Phys.-JETP5,1174 (1957)].

[13] E. B. Loginov and E. M. Terentjev, Sov. Phys. Crystallogr.30, 4 (1985), [Kristalografija 30,

10 (1985)].

[14] S. Kralj and T. J. Sluckin, Phys. Rev. E50, 2940 (1994).

[15] S. R. Renn and T. C. Lubensky, Phys. Rev. A38, 2132 (1988).

[16] E. Dubois-Violette, E. Guazzelli, and J. Prost, Phylosophical Magazine A48, 727 (1983).

[17] P. Oswald and M. Kleman, J. Physique Lettres (France)45, L319 (1984).

[18] I. Lelidis, M. Kleman, and J. L. Martin, Mol. Cryst. Liq. Cryst.330, 457 (1999).

[19] P. Oswald, P. Pieranski, F. Picano, and R. Holyst, Phys. Rev. Lett. 88, 015503 (2002), and

references therein.

[20] M. Kleman, J. Phys. (Paris) 35, 595 (1974).

[21] P.-G. de Gennes, C.R. Acad. Sci. (Paris)275, 939 (1972).

[22] A. Linhananta and D. E. Sullivan, Phys. Rev. A 44, 8189 (1991).

[24] N. D. Mottram, T. J. Sluckin, S. J. Elston, and M. J. Towler, Phys. Rev. E 62, 5064 (2000).

[25] P. C. Hohenberg and B. I. Halperin, Rev. Mod. Phys.49, 435 (1977).

[26] R. J. Bruinsma and C. R. Safinya, Phys. Rev. A43, 5377 (1991).

[27] H. R. Brand, P. K. Mukherjee, and H. Pleiner, Phys. Rev. E63, 016708 (2001).

[28] E. I. Kats, V. V. Lebedev, and S. V. Malinin, JETP95, 714 (2002), and references therein.

[29] R. F. Bruinsma and C. R. Safinya, Phys. Rev. A43, 5377 (1991), and references therein.

[30] H. Pleiner, Phys. Rev. A 37, 3986 (1988).

[31] A. Pargellis, N. Turok, and B. Yurke, Phys. Rev. Lett.67, 1570 (1991).

[32] A. Pargellis, P. Finn, J. W. Goodby, P. Panizza, B. Yurke, and P. E. Cladis, Phys. Rev. A

46, 7765 (1992).

[33] L. M. Pismen and B. Y. Rubinstein, Phys. Rev. Lett. 69, 96 (1992).

[34] G. Toth, C. Denniston, and J. M. Yeomans, Phys. Rev. Lett. 88, 105504 (2002).

[35] A. Bogi, P. M. Lagarde, I. Dozov, and M. Nobili, Phys. Rev. Lett.89, 225501 (2002).

[36] D. Svenˇsek and S. ˇZumer, Phys. Rev. E. 66, 021712 (2002).

[37] D. Svenˇsek and S. ˇZumer, Phys. Rev. Lett. 90, 155501 (2003).

[38] Z. Bradaˇc, S. Kralj, M. Svetec, and S. ˇZumer, Phys. Rev. E 67, 050702(R) (2003).

[39] see e. g. M. Kleman and O. D. Lavrentovich, *Soft matter physics, an introduction*

(Springer-Verlag, 2002), chap. 8, see chapters 8–10.

Figure caption

Fig.1 The geometry of the problem. The edge dislocations are initially separated by a
distance *L*0. The distances *Lx* and *Lz* describe the simulation cell volume. Bold lines
indicate the region over which calculations are carried out. Thin lines determine the smectic
layers. The two dots mark the centers of defects.

Fig.2 The order parameter profile of an isolated dislocation located at *z* = 0. Left panel:
smectic layer profile with contour plot of *η*(*x, z*) superimposed. Contours correspond to

Fig.3 Order parameter profile at different stages during the annihilation process. Left
panel: smectic layer profile with contour plot of *η*(*x, z*)superimposed. Contours correspond
to *η/ηb* = 0*.*95*,*0*.*8*,*0*.*6*,*0*.*4*,*0*.*2*,*0*.*05. Right panel: spatial variation of the order parameter
along the x-axis is shown at *z* = 0*, ξ,*2*ξ,*3*ξ,*4*ξ,*5*ξ,*6*ξ*.

(a) The late pre-collision regime, *L*= 5*ξ*;

(b) Exactly at the time of collision, *L*= 0;

(c) The early post-collision regime, *t*=*τ* and *η*(0*,*0)*/ηb* = 0*.*23.

Fig.4 The dynamics of the pre-collision regime.

(a) The*L*(*t*) dependence. Neglecting the initial anomalous dependence we roughly obtain

*L*∝p(*tc−t*). Care should be taken because the observed *L*(*t*) dependence on*L*0 is
due to memory effects. The results are obtained at a temperature where *ξ∼d*0.
(b) The dependence *v*(*L*) on a log-log plot. The law *v* *∝* 1*/L* would result in a straight

line with slope*−*1.

Fig.5 Pre-collision regime: the time evolution of the characteristic core size width in the
direction along the line connecting the defects and perpendicular to it. The diameters *ξx*
and *ξz*, characterizing the core shape, were measured in the *x* and*z* directions, respectively,
between opposite points at which *η*=*ηb/*2.

Fig.6 *η*(*x*= 0*, z* = 0) time evolution in the late pre-collision and post-collision regimes. .

Fig. 7 Influence of elastic anisotropy, nematic distortions and hydrodynamics on the *L*(*t*)
dependence. In all cases *L*0 = 60*ξ*. a) *Ck/C⊥* = 1, *κn* = *∞,* the solid line; b) *Ck/C⊥* = 5,

*κn* = *∞*, the dashed line; c) *Ck/C⊥* = 1, *κn* = 0, the dotted line; d) *Ck/C⊥* = 1, *κn*
= *∞*, addition of advection terms, the dash-dotted line. The ratio *ak/a⊥* = 4, typical for